- Open Access
Calotropis gigantea assisted green synthesis of nanomaterials and their applications: a review
Beni-Suef University Journal of Basic and Applied Sciences volume 9, Article number: 14 (2020)
Nanotechnology has been receiving wonderful impetus in the current emerging technological era by opening a pool of scientific ideas to compete with the daily challenges of developing technology. So far, numerous properties and countless applications of nanomaterials have been explored which have been even proved to be based on characteristic shape, size, surface area and surface chemistry.
By the time, several attempts have been made for green synthesis of nanomaterials, using plant extracts. Calotropis gigantiea (L.) R. Br is the plant belonging to Apocynaceae, have been screened and proved to possess various pharmacological activities, due to different polar phytochemicals like flavonoids, lignans and terpenoids. This review focus on phytochemicals so far reported from different parts of the plant; pharmacological activities exhibited; green synthesis of nanomaterials, particularly metallic nanoparticles green synthesised by facilitating reaction of metallic ion donor molecule/salt and aqueous extract of leaves or flowers of C. gigantiea and their biological or non-biological applications. The use of C. gigantea in the fabrication of nanomaterials is an eco-friendly and safe approach. Secondary metabolites present act as a stabilizing agent for nanomaterials. Cadmium sulphide, titanium dioxide, nickel and nickel oxide nanoparticles synthesised using C. gigantea exerted better anti-microbial action, compared to extracts. Nanoencapsulated magnesium oxide nanoparticles avoided biochemical degradation of MgO; increase its bioavailability and proved beneficial in type II diabetes mellitus. Cupric oxide nanoparticles got applied in dye-sensitised solar cell. Silver nanoparticles showed better cytotoxicity in HeLa cells. Biomaterial-supported zero-valent iron and stannic oxide nanoparticles proved to have utilities in water purification. Green synthesised Eu3+ doped Y2SiO5 nanophosphors had significant chromaticity coordinates and average correlated colour temperature, hence find application in displays.
Variety of nanomaterials including nanoparticles and nanophophors could successfully be biosynthesised using Calotropis gigantean extract or its latex. These green synthesised nanomaterials have several applications in the healthcare system and technology.
Nanotechnology has gained marvellous impetus in today’s rapidly emerging technological era by generating a wealth of scientific concepts to tackle with daily challenges of developing technology . The nanomaterials have been proved to possess countless applications and physicochemical properties [2, 3] which are exerted due to their characteristic size, shape, area and surface chemistry . These features of nanomaterials enable them to be highly reactive and thereby more attractive for researchers . These nanomaterials may exist in the form of nanotubes, nanocrystals, nanoparticles, nanospheres, nanophosphors or even in their combination, i.e. nanohybrids. In the recent era, different metallic nanoparticles are gaining research interest in material chemistry due to their unique catalytic, electrical and optical characteristics. These nanomaterials could be conjugated with various functional biomolecules such as antibodies, ligands, and drugs of interest for biomedical applications.
Manufacturing of nanomaterials
Depending upon the particular type, nanomaterials can be manufactured by one of the two approaches: bottom-up and top-down. The bottom-up approach involves placing of atom by atom or molecule by molecule; which can be achieved by chemical synthesis, self-assembly and positional assembly. Top-down strategy implicates etching, milling or grinding of a larger piece of material to be converted to its nanoform. In this approach, complex devices are used, requiring high energies and producing more wastes. Hence, bottom-up strategies are preferred where atoms or molecules are get arrange themselves into ordered nano-structures by physical and/or chemical interactions.
As far as Calotropis gigantea is concerned, different research articles pertaining to a variety of aspects, right from primary microscopic features of different parts, their preliminary phytochemical evaluation, various pharmacological screening and application of its extracts in green synthesis of nanomaterials have been published. Most of these research articles are available on internationally reputed, well-recognised search engines like ScienceDirect (http://www.sciencedirect.com), Wiley Online Library (http://onlinelibrary.wiley.com), Springer (http://linnk.springer.com), Taylor and Francis (http://www.tandfonline.com), Nature (www.nature.com) and PubMed (http://www.ncbi.nlm.nih.gov>pubmed). This review highlighted the phytochemicals reported to be present in a given part of plant Calotropis gigantea which could be claimed to be present in extract using which several successful attempts of green synthesis of nanomaterials were made. This review throws the light on the method used for their green synthesis as well as the biological/pharmacological and non-biological applications of these nanomaterials.
Botanical description of Calotropis gigantea
The word Calotropis was derived from the Greek word “Kalos” meaning beautiful and “tropis” meaning keel, referring to the shape of the coronal scales. Calotropis gigantea (crown flower) (Fig. 1) is a large shrub or small tree, belonging to family Asclepiadeae, characterised by the presence of a smooth and soft tomentum on stems and lower leaf surfaces, calyx lobes with many glands at the base, broadly campanulate corollas, and coronal scales with a recurved spur at the base. Among various species, this one, C. gigantea is an Asiatic, occurring widely throughout the Indian subcontinent, southern China, South East Asia and has also been introduced into New Guinea and Hawaiian islands .
Phytochemical composition of Calotropis gigantea
Over time, variety of secondary metabolites have been reported to be isolated from different parts of Calotropis gigantea and structurally elucidated.
As per Lhinhatrakool T, Sutthivaiyakit S. , the leaves of C. gigantea contain pinoresinol, medioresinol, uzarigenin, calotropin, calactin, calacitnic acid, calacitnic acid methyl ester, 19-carboxyl-calacitnic methyl ester, drummondol, 15b-hydroxycalotrin, the C-11 bicylic lactone, norisopenoid, the rare diphenyl furfuran lignan and salicifoliol. Seeka and Sutthivaiyakit  isolated 15-β-Hydroxycardenolides and 16-α-hydroxycalactinic acid methyl ester while Nguyen et al.  isolated a lignan, 9′-methoxypinoresinol and two new glycosylated 5-hydroxymethylfurfurals, calofurfuralside A and calofurfuralside B from the leaves of C. gigantea. Di-(2-ethylhexyl) Phthalate and anhydrosophoradiol-3-acetate were isolated from flower . Sen et al.  isolated flavonol glycosides, isorhamnetin-3–0-[2-O–β-D-galactopyranosyl–6–O–α–L-rhamnopyranosyl]–β-D-glucopyranoside, isorhamnetin-3-O-rutinoside, isorhamnetin–3–0-glucopyranoside and taraxasteryl acetate from aerial parts of C. gigantea. The fixed oil separated from seeds of C. gigantea was reported to contain lauric acid, myristic acid, palmitic acid, palmitoleic acid, stearic acid, oleic acid, linoleic acid, linolenic acid, arachidic acid and behenic acid (book chapter). These fatty acids are also present in the form of mono-, di-, and tri-acyl glycerols at the surface of and internal to leaves . Terpenoids derivatives like pentacyclic Triterpenic Esters and lupeoul acetate were isolated from the roots of C. gigantea .
Pharmacological potential of Calotropis gigantea
Calotropis gigantea is a notorious weed, so far not cultivated commercially. Still, the plant has been screened for different pharmacological activities, in the form of extract of any part, isolated compound or latex, using different scientifically accepted in-vivo or in-vitro models . Based on phytochemicals present, different parts of Calotropis gigantea were reported to possess different pharmacological activities (Table 1).
Green synthesis of nano-structures and their applications
Several researchers tested the hypothesis which was based on nanostructures if synthesised using C. gigantea or its latex, could have improvement in pharmacological potential exhibited by different extracts prepared using different parts of C. gigantea or latex collected; or else, these nanomaterials could be used in non-biological applications like those in the field of energy or television displays (LEDs and LCDs).
Cadmium sulphide nanoparticles
In 2017, Ayodhya and Veerabhadram  synthesised cadmium sulphide nanoparticles using aqueous extract of leaves of C. gigantea. The extract was further mixed with 40 mL of 1 mM of cadmium acetate and 40 mL of 1 mM of sodium sulphide to obtain spherical CdS NPs. CdS NPs were then characterised for their morphology, stability and particle size; photocatalytic activity was studied under sunlight irradiation using MB and EY dyes. The XRD pattern of CDs NPs exhibited three prominent peaks at 2θ values of 26.4°, 43.4° and 51.6°; corresponding to the (111), (220) and (311) diffraction planes of cubic crystals. The average particle size of CdS NPs was found to be 12 nm. The nanophase and quantum confinement nature of the synthesised CdS NPs was indicated by enhancement of the optical band gap of 2.42 eV. It was also observed that as in particle size decreases, the energy of separation between the ground and excited electronic states increases; resulting in a blue shift in absorption. The capping effects and functional groups of C. gigantea leaf extract phytochemicals on CdS NPs surfaces were investigated by ATR–FTIR. The longevity of CdS NPs was tested by recycling the photocatalyst used in the photocatalytic degradation of MB and EY dyes under 60 min of sunlight irradiation. The result indicated that the CdS catalysts are fairly photostable and practically applicable. It was claimed that electron-donating functional groups of phytochemical present in aqueous extract of C. gigantea leaves are responsible for the stability of CdS NPs and the reduction of both dyes. Further, CdS NPs were evaluated for antimicrobial activity and compared with that exerted by core C. gigantea leaves extract. In the culture of bacteria, E. coli, P. aeruginosa, S. aureus and B. thuringiensis; and fungi, A. niger and C. albicans; zone of inhibition obtained with CdS NPs were 4 to 6 times wider than those obtained with C.gigantea leaves extract. About anti-fungal activity, it was claimed that CDs NPs got saturated and adhered to fungal hypha and to disrupt them.
Magnesium oxide nanoparticles
As such oral magnesium supplements are consumed to increase insulin sensitivity and reducing the risk of the onset of type 2 diabetes. This is because magnesium is an important co-factor/prosthetic group for phosphorylation causing enzymes like tyrosine-kinase, playing a significant role in insulin signalling pathway. But commonly available supplement, magnesium oxide, MgO has poor oral bioavailability and thereby may get decomposed by gastric acid. Hence, with the hypothesis that nanoencapsulated magnesium oxide nanoparticles (MgO NPs) can avoid all these biochemical degradation of MgO and increase its bioavailability. Carried out the synthesis of MgO NPs using aqueous extract of C. gigantea and their nano-encapsulation into polymer polyvinylpyrrolidone (PVP) or Eudragit L . Aqueous extract of C. gigantea leaves played a significant role in the formation and stabilization of MgO NPs. The MgO NPs so formed were then encapsulated by following conventional emulsion solvent evaporation method where 10 mg of MgO NPs and 20 mg of PVP or 20 mg of Eudragit L were dissolved in 10 mL of ethanol. Then, about 10 ml of distilled water containing Tween80 (2%, w/w) or 10 mL liquid paraffin containing sorbitan sesquioleate (2%, w/w) was added as the emulsifier. Then, these mixtures were heated to 80C and stirred at an agitation speed of 250 rpm on a magnetic stirrer until ethanol was fully disappeared and that nanosuspensions were centrifuged at 13200 rpm for 20 mins to get PVP-MgO NPs or Eudragit L-MgO NPs. The average size of MgO NPs obtained was 48.38 nm while their crystallite size was 8 nm. When encapsulated by emulsion solvent evaporation, PVP-MgO NPs and Eudragit L-MgO NPs, particle size increased to 96.65 and 53.37 nm, respectively. Eudragit L-MgO NPs had higher stability. Drug entrapment efficiency (%) and drug loading (%) for Eudragit L-MgO NPs were found higher than those for PVP-MgO NPs. It was also observed that drug release pattern of Eudragit L-MgO nanoparticles was as per Fickian diffusion mechanism and coincided well with the Weibull model.
Nickel and nickel oxide nanoparticles
Nickel (Ni) is the transition metal, exhibiting magnetism and catalytic properties. Nickel nanoparticles (NiNPs) have been proved to adsorb environmentally hazardous dyes and inorganic pollutants . They also possess good antibacterial and anti-inflammatory activities . On the other hand, its oxide form NiO has cubic crystal lattice structure with p-type semiconductor properties. Nanoparticles of NiO (NiO-NPs), due to their electron transfer capability with their own high chemical stability and super-capacitance properties ; they exhibit technical applications in battery cathodes, fuel cells, electrochromic films, magnetic materials, optical fibres and gas sensors . Considering these potential applications, Din et al.  fabricated Ni-NPs and NiO-NPs using hydro-methanolic (40% methanol) extract of freshly collected leaves of C. gigantea. In UV/vis spectrum, sharp exciton absorption was positioned at 415 nm, suggested that C. gigantea extract assisted green synthesised NiO NPs were stable. The FT-IR spectra of both Ni and NiO NPs did not show a peak around 1000–1100 cm−1 while peak for O–H bond got reduced in Ni NPs FTIR spectrum and almost completely reduced in NiO NPs FTIR spectrum; suggesting the important role of alcohols and halogens in metal ion reduction. Amines also played role as a capping agent in the fabrication of Ni-NPs. As per the results of XRD-analysis the particle size of Ni-NPs was in the range of 20–40 nm while that may higher up to 60 nm for NiO NPs. Further, on antimicrobial screening of Ni and NiO-NPs against Pseudomonas auruginosa, these were found equally potent, compared to Chloramphenicol.
Titanium dioxide nanoparticles
Infection by tick parasites like Rhipicephalus microplus and Haemaphysalis bispinosa is major hindrance in having and sustaining new generations of cattle. To have a scientific check for hypothesis that titanium dioxide nanoparticles (TiO2 NPs) could be exhibiting significant acaricidal activity, Marimuthu et al.  attempted the green synthesis of TiO2 NPs using aqueous extract C. gigantea flowers and morphologically characterised. XRD pattern of TiO2 NPs showed diffraction peaks at 2θ values of 27.33°, 35.83°, 43.87°, 54.02°, 56.39°, 66.64° and 74.07° could be assigned to the (110), (101), (210), (211), (220), (301) and (320), respectively; indicating faced centre cubic lattice structure of TiO2 NPs. SEM showed their spherical shape with particle size ranging between 160 and 220 nm . also evaluated TiO2 NPs against R. microplus and H. bispinosa by filter paper impregnated bioassay protocol. Researchers found that LC50 values shown by aqueous extract of flowers and TiO (OH)2 solution are around four times higher than those shown by TiO2 NPs, indicating TiO2 NPs can be used to treat the tick parasitic infection in cattle.
Cupric oxide nanoparticles
To fulfil the increasing demands for energy, the development of photovoltaic technology especially, dye-sensitised solar cells (DSSCs) are getting importance and research interest. Cupric oxide (CuO) is a p-type semiconductor with narrow bandgap (Eg 1.2 eV) and material for the fabrication of various electronic and optoelectronic devices . Therefore, in the fabrication of DSSCs, CuO NPs have been considered as an alternative counter electrode material. CuO NPs can also be used in making high-temperature superconductors  gas sensors  and giant magnetoresistance materials . When incorporated into coatings, plastics and textiles, CuO NPs acts as anti-fouling and antimicrobial . Considering these technical applications, Sharma et al. , synthesised CuO NPs from Cupric Nitrate added to aqueous extract of C. gigantea leaves and fabricated CuO nanoparticles based counter electrode that to be used in DSSC. Initially, the formation of nanostructures was confirmed by the increased bandgap of 1.86 eV. In XRD analysis, several intense peaks at 2θ values of 32.4, 35.5, 38.7, 48.7, 53.4, 58.3, 61.5, 66.2, 68.0, 72.4 and 75.2o, were obtained, which could be assigned to (110), (002), (111), (202), (020), (202), (113), (311), (113), (311) and (222), respectively; indexing as typical monoclinic structure of CuO NPs. TEM analysis revealed the spherical shape of CuO NPs with a particle size up to 20 nm. The cyclovoltametric measurement exposed that CuO NPs-based material showed to be a reasonably good platform for the reduction of triiodide ions in redox electrolyte, signifying its good electrocatalytic activity towards the iodide ions (Fig. 2). Kumari et al.  attempted synthesis of CuO NPs by the addition of floral extract of C. gigantea to1 mM CuCl2 solution and characterised by advanced techniques. The hydrodynamic diameter of synthesised CuO NPs showed the diameter of 109 ± 11 nm. The zeta potential of CuO NPs was found to be − 34 ± 12 mV. The XRD peaks were observed at 2θ values of 32.5, 35.5, 38.7, 48.7, 53.0, 58.2, 63.4, 66.2 and 68.1 corresponding to (110), (002), (111), (202), (020), (202), (113), (311) and (113), respectively. The result indicated a typical monoclinic structure of CuO NPs . also explained the mechanism of biosynthesis of CuO NPs, according to which phytochemicals having hydroxyl groups played a significant role in reducing copper (II) chloride to copper hydroxide (Cu (OH)2). Further, Cu (OH)2 got reduced to CuO NPs which were capped and stabilised by phytochemicals present in the floral extract of C. gigantea extracted in an aqueous medium.
The toxicity of CuO NPs was evaluated by determining their effect on physiological and morphological changes in Zebrafish embryo. Surprisingly, the hatching rate was found higher in the case of embryos exposed to CuO NPs as compared to the commercial one. It was also observed that CuO NPs got accumulated at chorion, yolk sac and skin surface of 24, 48 and 72 h post-fertilization (hpf).
To determine the effect of synthesised CuO NPs in Zebrafish embryos at the cellular level, ROS induction and apoptosis were analysed in embryos after 72 hpf of treatment with the help of flow cytometry and Acridine orange staining-based fluorescent microscopy.
Zinc oxide nanoparticles
Two successful attempts were made for green synthesis of zinc oxide nanoparticles (ZnO NPs) using C. gignatea. Vidya et al.  used aqueous extract of C. gignatea leaves. They got hexagonal ZnO NPs ranging in size of 30–35 nm. Panda et al.  employed milky latex obtained by making an incision on the intact branches of C. gignatea and precursor zinc acetate; and carried out alkaline precipitation method. XRD pattern showed 13 characteristic diffraction peaks of (100), (002), (101), (102), (110), (103), (200), (112), (201), (004), (202, 104) and (203), observed at 2θ angles; 31.77°, 34.42°, 36.25°, 47.54°, 56.6°, 62.86°, 66.38°, 67.96°, 69.09°, 72.56°, 76.95°, 81.37° and 89.6°, respectively, reflecting wurtzite crystalline structure of ZnO NPs. C. gigantea milky latex-based ZnO NPs induced oxidative stress in DNA damage as determined by Comet assay in the root assay system of L. sativus, which was found comparable to that induced by the commercially available ZnO NPs-S (S for Sigma-Aldrich, St. Louis, MO, USA).
Rajkuberan et al.  synthesised silver nanoparticles (AgNPs) using freshly collected milky white latex of C. gigantea. Latex was first converted to 3% aqueous extract and then about 1 ml was added to 9 ml of 2 mM silver nitrate, AgNO3. Then, AgNps were characterised by UV-Vis absorbance spectroscopy, FTIR analysis, X-ray diffraction, FeSEM and TEM techniques; and evaluated for their antibacterial activity against Shigella and P. aeruginosa; and cytotoxicity against HeLa cells. XRD pattern showed diffraction peaks at (111), (101), (103) and (105) corresponded to 2θ values of 38.12, 47.08, 57.93 and 76.71°, respectively depicted that AgNPs had mixed phase of cubic and hexagonal structures. As per Debye–Scherrrer’s equation, the average particle size was calculated as 12 nm. About antimicrobial activity, it was observed that zone of inhibition created by lowest concentration 10 μl of AgNPs was 2 to 3 times higher in diameter than those created by 3% aqueous latex extract. Cytotoxicity exerted by these AgNPs against HeLa cells was also significant with LC50 of 91.3 μg; however, that with 3% aqueous latex extract was found to be 311 μg.
Iron oxide nanoparticles and biomaterial-supported zero-valent iron nanoparticles
Jain et al.  employed aqueous extract of C. gigantea for phytofacation of iron oxide nanoparticles. The XRD pattern of the product can be clearly pointed to the face-centered cubic spine structure of iron oxide nanoparticles with a lattice parameter of a = 8.393 Å and a size ranging between 3 and 6 nm; exposing that reduction of Fe3+ by C. gigantea aqueous extract leads to FeO NPs as the final product. Further, in 2018, zero-valent iron nanoparticles (ZVIN) were synthesised by green eco-friendly method using aqueous extract of C. gigantea flowers and characterised by UV-Vis, FT-IR, XRD, SEM, and EDX . The ZVIN so synthesised were spherical in shape and 50–90 nm in size. From the FT-IR and UV-visible spectrum, Sravanthi et al. 2018 concluded that polyphenols present in the flower extract were responsible for the reduction and stabilization of ZVIN. Then, they proved the effectivity of ZVIN in controlling water pollution by adsorptive removal of organic waste such as methylene blue (synthetic dye) (Fig. 3) and aniline (aromatic primary amine) from contaminated water.
Tin oxide/stannic oxide nanoparticles
Tin oxide/stannic oxide (SnO2) is one of the n-type semiconductor having a bandgap of 3.6 eV, thereby used in photoconductive and photochemical device in liquid crystal display and lithium-ion batteries; and transparent conductive electrode for solar cells, gas sensors . Because of the high surface to volume ratio, SnO2 NPs exhibit increased sensitivity and adsorption and can be used as photocatalyst . Considering this significance, Bhosale et. al.  attempted the green synthesis of SnO2 NPs by the addition of dilute aqueous extract of leaves to 0.05 M solution of tin chloride (SnCl4 ·5H2O) with constant stirring. They claimed that tin chloride reacted with polyphenols present in the extract and following calcination, they got SnO2 NPs with spherical morphology of an average size of 35 nm. In XRD pattern, the peaks at 2θ values of 26.5°, 34°, 37.9°, 51.7°, 54.4°, 57.7°, 61.7°, 64.8°, 71.3° and 78.5° were associated with (110), (101), (200), (211), (220), (002), (310), (301), (202) and (222) planes, respectively, proving the formation of SnO2 NPs with tetragonal structure. Then, Bhosale et al. 2018 also explained the plausible mechanism for the formation of SnO2 NPs, according to which SnCl4.5H2O salt solution on mixing with C. gigantea leaf extract, Sn4+ ions form a complex with hydroxyl groups. The complex so formed got decomposed on calcination. Polyphenolic molecules then kept Sn4+ cations together forming SnO2 NPs. Taking dye methyl orange as a model pollutant under UV-light, its degradation was further tested as a function of photocatalytic potential of the synthesised SnO2 NPs (Fig. 4).
Eu3+ doped Y2SiO5 nanophosphors
During the last decade, white light-emitting diodes (WLEDs), due to high efficiency, energy-saving, long lifetime, safety and environmental protection have fascinated a lot of research interest in the solid-state lighting . White light was obtained by the foremost technique involving the mixing ultraviolet (UV) LED chip with tricolour phosphors  but the lack of appropriate red phosphors decreased colour rending index (CRI). So far newly designed red phosphor, Y2O2S: Eu3+ has shown low efficiency and poor chemical stability. Therefore, Ramakrishna et al.  accepted this challenge of developing a new red phosphor with sufficiently high luminous efficiency and fabricated red-emitting Eu3+ doped Y2SiO5 nanophosphors using C. gigantea latex, Yttrium nitrate (Y (NO3)3, Europium nitrate (Eu (NO3)2, H2O and NaCl. The Eu3+ doped Y2SiO5 nanophosphors so obtained were irregular shape with an average size of 32 nm which was found decreasing on the increasing concentration of (Eu (NO3)2. Determination of optical properties of Eu3+ doped Y2SiO5 nanophosphors was based on emission spectra and Judd–Ofelt theory. It was observed that there is ionic bonding between Eu3+ ions and host; and assembled in symmetrical in coordination structure surrounding the (rare earth) RE ion. This newly synthesised phosphor exhibited admirable International Commission on Illumination (CIE) chromaticity coordinates (0.5866, 4026) and average correlated colour temperature CCT value 2018.5 K. Hence, researchers claimed that these Eu3+ doped Y2SiO5 nanophosphors could have potential application in the fabrication of near-ultraviolet excited white light-emitting diodes (Fig. 5).
Calotropis gigantea (Asclepiadeae) is the plant having several well-proved pharmacological actions. Several types of nanomaterials have been synthesised following green approach using aqueous extract of different parts of C. gigantea; evaluated for different pharmacological activities and potential were compared that with extracts. Nanomaterials tried to get synthesised include nanoparticles and nanophophors. Importantly, green synthesis of nanoparticles has upsurge as new nanobiotechnology to produce eco-friendly and cost-effective synthetic processes for highly stable nanoparticles which emerges as a safer alternative to conventional methods. These nanoparticles were proved to have better antimicrobial action against both animal and plant infecting pathogens and utilities in controlling the water pollution by adsorbing or precipitating pollutants, demonstrated using dyes and other organic compounds. Nanophosphors have been extensively investigated during the last decade due to their application potential for various high-performance displays and devices.
Availability of data and materials
- Ag NPs:
Correlated colour temperature
- CdS NPs:
Cadmium sulphide nanoparticles
Colour rending index
- CuO NPs:
Cupric oxide nanoparticles
Fourier transform-infrared spectroscopy
Nickel oxide nanoparticles
Scanning electron microscopy
- SnO2 NPs:
Tin oxide/stannic oxide nanoparticles
Transmission electron microscopy
- TiO2 NPs:
Titanium dioxide nanoparticles
- ZnO NPs:
Zinc oxide nanoparticles
Zero-valent iron nanoparticles
Antonietti M (2016) Small is beautiful: challenges and perspectives of nano/meso/microscience. Small. 12(16):2107–114
Na Y, Yang S, Lee S (2014) Evaluation of citrate-coated magnetic nanoparticles as draw solute for forward osmosis. Desalination 347:34–42
Davar F, Fereshteh Z, Salavati-Niasari M (2009) Nanoparticles Ni and NiO: synthesis, characterization and magnetic properties. J Alloys Compd 476(1–2):797–801
Kreyling WG, Semmler-Behnke M, Chaudhry Q (2010) A complementary definition of nanomaterial. Nano Today 5(3):165–168
Krishnamurthy N, Vallinayagam P, Madhavan D (2014) Engineering chemistry. PHI Learning Pvt Ltd, Delhi
Rahman MA, Wilcock CC (1991) A taxonomic revision of Calotropis (Asclepiadaceae). Nord J Bot 11(3):301–308
Lhinhatrakool T, Sutthivaiyakit S (2006) 19-nor- and 18, 20- epoxycardenolides from the leaves of Calotropis gigantea. J Nat Prod 69:1249–1251
Seeka C, Sutthivaiyakit S (2010) Cytotoxic Cardenolides from the leaves of Calotropis gigantea. Chem Pharm Bull 58(5):725–728
Nguyen KDH, Dang PH, Nguyen HX, Nguyen MTT, Awale S, Nguyen NT (2017) Phytochemical and cytotoxic studies on the leaves of Calotropis gigantea. Bioorg Med Chem Lett 27:2902–2906
Habib MR, Karim MR (2009) Antimicrobial and cytotoxic activity of Di-(2-ethylhexyl) phthalate and anhydrosophoradiol-3-acetate isolated from Calotropis gigantea (Linn.) flower. Mycobiology 37(1):31–36
Sen S, Sahu NP, Mahato SB (1992) Flavonol glycosides from Calotropis gigantean. Phytochemistry 31(8):2919.2921
Lakshminarayana G, Rao KS, Pantulu AJ, Gupta DR (1988) Surface and Internal Lipids of Calotropis gigantea L. Leaves. Fat Sci Technol 90(Jahrgang Nr.2):65–67
Ali M.; Gupta J; Indian J. Chem., Sect. B: Org. Chem. Incl. Med. Chem. 38 (1999) 7, 877–881;
Kadiyal M, Ponnusankar S, Elango K (2013) Calotropis gigantiea (L.) R. Br (Apocynaceae): a phytochemical and pharmacological review. J Ethnopharmacol 150(1):32–50
Pathak AK, Argal A (2007) Analgesic activity of Calotropis gigantea flower. Fitoterapia 78:40–42
Habib MR, Karim MR (2013) Effect of anhydrosophoradiol-3-acetate of Calotropis gigantea (Linn.) flower as antitumoric agent against Ehrlich’s ascites carcinoma in mice. Pharmacol Rep 65:761–767
Ishnava KB, Chauhan JB, Garg AA, Thakkar AM (2012) Antibacterial and phytochemical studies on Calotropis gigantia (L.) R. Br. Latex against selected cariogenic bacteria. Saudi J Biol Sci 19:87–91
Pattnaik PK, Dattatreya KD, Chhatoi H, Shahbazi S, Ghosh G, Kuanar A (2017) Chemometric profile & antimicrobial activities of leaf extract of Calotropis procera and Calotropis gigantea. Nat Prod Res 31(16):1954–1957
Chitme HR, Chandra R, Kaushik S (2005) Evaluation of antipyretic activity of Calotropis gigantea (Asclepiadaceae) in experimental animals. Phytother Res 19:454–456
Habib MR, Karim MR (2011) Evaluation of antitumour activity of Calotropis gigantea L. root bark against Ehrlich ascites carcinoma in Swiss albino mice. Asian Pac J Trop Med 4:786–790
Argal A, Pathak AK (2006) CNS activity of Calotropis gigantea roots. J Ethnopharmacol 106:142–145
Ghule SD, Vidyasagar G, Bhandari A, Sharma P, Gunjal AP (2014) CNS activity of leaves extract of Calotropis gigantea. Asian Pac J Trop Dis 4(Suppl 2):S902–S905
Taylor P, Arsenak M, Abad MJ, Fernández A, Milano B, Gonto R, Ruiz MC, Fraile S, Taylor S, Estrada O, Michelangeli F (2012) Screening of Venezuelan medicinal plant extracts for cytostatic and cytotoxic activity against tumor cell lines. Phytother Res 24(4):530–539
Wong SK, Lim YY, Abdullah NR, Nordin FJ (2011) Assessment of antiproliferative and antiplasmodial activities of five selected Apocynaceae species. BMC Complement Altern Med 11(3):1–8
Parhira S, Zhu G, Chen M, Bai L, Jiang Z (2016) Cardenolides from Calotropis gigantea as potent inhibitors of hypoxiainducible factor-1 transcriptional activity. J Ethnopharmacol 194:930–936
Deshmukh PT, Fernandes J, Akarte A, Toppo E (2009) Wound healing activity of Calotropis gigantea root bark in rats. J Ethnopharmacol 125:178–181
Srivastava SR, Keshri G, Bhargavan B, Singh C, Singh MM (2007) Pregnancy interceptive activity of the roots of Calotropis gigantea Linn. In rats. Contraception 75:318–322
Rajesh R, Gowda CDR, Nataraju A, Dhananjaya BL, Kemparaju K, Vishwanath BS (2005) Procoagulant activity of Calotropis gigantea latex associated with fibrin (ogen) olytic activity. Toxicon 46:84–92
Ayodhya D, Veerabhadram G (2017) One-pot green synthesis, characterization, photocatalytic, sensing and antimicrobial studies of Calotropis gigantea leaf extract capped CdS NPs. Mat Sci Engineering B 225:33–44
Hii YS, Jaison Jeevanandam J, San Chan YS (2018) Plant mediated green synthesis and nanoencapsulation of MgO nanoparticle from Calotropis gigantea: Characterisation and kinetic release studies. Inorg Nano-Met Chem 48 (2018):620–31
Pandian CJ, Palanivel R, Dhananasekaran S (2015) Green synthesis of nickel nanoparticles using Ocimum sanctum and their application in dye and pollutant adsorption. Chin J Chem Eng 23(8):1307–1315
Angajala G, Radhakrishnan S (2014) A review on nickel nanoparticles as effective therapeutic agents for inflammation. Inflamm Cell Signal 1(3):1–8
Thema F, Manikandan E, Gurib-Fakim A, Maaza M (2016) Single phase Bunsenite NiO nanoparticles green synthesis by Agathosma betulina natural extract. J Alloys Compd 657:655–661
Borgström M, Blart E, Boschloo G, Mukhtar E, Hagfeldt A, Hammarström L, Odobel F (2005) Sensitized hole injection of phosphorus porphyrin into NiO: toward new photovoltaic devices. J Phys Chem B 109(48):22928–34
Din MI, Nabi AG, Rani A, Aihetasham A, Mukhtar M (2018) Single step green synthesis of stable nickel and nickel oxide nanoparticles from Calotropis gigantea: catalytic and antimicrobial potentials. Environ Nanotechnol Monit Manag 9:29–36
Marimuthu S, Rahuman AA, Jayaseelan C, Kirthi AV (2013) Acaricidal activity of synthesized titanium dioxide nanoparticles using Calotropis gigantea against Rhipicephalus microplus and Haemaphysalis bispinosa. Asian Pac J Trop Med 6:682–688
Kumar RV, Elgamiel R, Diamant Y, Gedanken A, Norwig J (2001) Langmuir 17:1406–1410
Malandrino G, Condorelli GG, Lanza G, Fragala IL, Alloys J (1997) Compd 251:314–316
Ishihara T, Higuchi M, Takagi T, Ito M, Nishiguchi H, Takita T (1998) J Mater Chem 8:2037–2042
Liu X, Bi N, Feng C, Or SW, Sun Y, Jin C, Li W, Xiao F, Alloys J (2014) Comp 587:1–5
Apostolov AT, Apostolova IN, Wesselinowa JM (2014) Solid State Commun 192:71–74
Sharma JK, Akhtar MS, Ameen S, Srivastava P, Singh G (2015) Green synthesis of CuO nanoparticles with leaf extract of Calotropis gigantea and its dye-sensitized solar cells applications. J Alloys Compd 632:321–325
Kumari P, Panda PK, Jha E, Kumari K, Nisha K, Mallick MA, Verma SK (2017) Mechanistic insight to ROS and Apoptosis regulated cytotoxicity inferred by green synthesized CuO nanoparticles from Calotropis gigantea to embryonic Zebrafish. Sci Rep 7:16284
Vidya C, Hiremath S, Chandraprabha MN, Antonyraj MAL, Venu GI, Jain A, Kokil BK (2013) Green synthesis of ZnO nanoparticles by Calotropis gigantea. Int J Curr Engineering Technol (1):118–20
Panda KK, Golari D, Venugopal A, Achary VMM, Phaomei G, Parinandi NL, Sahu HK, Panda BB (2017) Green synthesized zinc oxide (ZnO) nanoparticles induce oxidative stress and DNA damage in Lathyrus sativus L. Root Bioassay System. Antioxidants 6:35
Rajkuberan C, Sudha K, Sathishkumar G, Sivaramakrishnan S (2014) Antibacterial and cytotoxic potential of silver nanoparticles synthesized using latex of Calotropis gigantea L. Spectrochimica Acta Part A: Mol Biomol Spectroscopy 136B:924–30
Jain D, Rathore KS, Jain R, Singh H, Kachhwaha S, Kothari SL (2013) Phytofabrication of Iron oxide nanoparticles using Calotropis gigantea L. Adv Sci Focus 4(1):318–321
Sravanthi K, Ayodhya D, Swamy PY (2018) Green synthesis, characterization of biomaterial-supported zero-valent iron nanoparticles for contaminated water treatment. J Analytical Sci Technol 9:3
Naje AN, Norry AS, Suhail AM (2013) IJIRSET 2:7068
Suwarnkar MB, Kadam AN, Khade GV, Gavade NL, Garadkar KM (2016) J Mater Sci Mater Electron 27:843
Bhosale TT, Shinde HM, Gavade NL, Babar SB, Gawade VV, Sabale SR, Kamble RJ, Shirke BS, Garadkar KM (2018) Biosynthesis of SnO2 nanoparticles by aqueous leaf extract of Calotropis gigantea for photocatalytic applications. J Mater Sci. volume 8
Yu R, Noh H, Moon B, Choi B, Jeong, Lee H, Jang K, Yi S (2014) J Lumin 145:717–722
Liang CH, Chang YC, Chang YS (2008) Appl Phys Lett 93:211902
Ramakrishna G, Nagabhushana H, Daruka PD, Vidya YS, Sharma SC, Anantharaju KS, Prashantha SC, Choudhary N (2016) Spectroscopic properties of red emitting Eu3+ doped Y2SiO5 nanophosphors for WLED’s on the basis of Judd-Ofelt analysis: Calotropis gigantea latex mediated synthesis. J Lumin 181:153–63
The author of this manuscript is thankful to Dr.(Mrs.) Anagha M. Joshi, Principal, SCES’s Indira College of Pharmacy, Pune, for her encouragement and also for providing internet and library facilities at the college premises to access the articles and books to carry out this review.
Ethics approval and consent to participate
Consent for publication
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Patil, S.P. Calotropis gigantea assisted green synthesis of nanomaterials and their applications: a review. Beni-Suef Univ J Basic Appl Sci 9, 14 (2020). https://doi.org/10.1186/s43088-020-0036-6
- Calotropis gigantea
- Metal nanoparticles
- Zero-valent iron nanoparticles
- Eu3+ doped Y2SiO5 nanophosphors